INDUSTRIAL AND ENGINEERIKG CHEMISTRY
cent catechol would prove more serviceable for a particular application such as a tire tread or a conveyor belt cover than the same vulcanizate without these modifying agents. However, for a complete evaluation of such a compound it would be necessary to study the effect of the modifying agents on the stability of the unvulcanized compound and the effect on the physical properties of the vulcanizate a t elevated temperatures. The fact that the properties of a given vulcanizate can be so varied opens up a new field of compounding research since it is obvious that other combinations of these or other chemicals may be expected to produce similar 01more desirable results.
The carbon black in the compounds is a type commonly used in the rubber industry, but it should not be inferred that the varieties of carbon black that are found to be best in the compounding of rubber to meet definite physical requirements are necessarily best for the compounding of neoprene to meet the same requirements.
Literature Cited (1) “Compounding Ingredients for Rubber,” New York, Bill Bros. Publishing Corp., 1936. ( 2 ) Lessig, E. T., IND. EKG.cHEM., Anal. Ed., 9, 582 (1937). (3) Winkelmann, Proc. Am. SOC.Testing Materials, 31, 897 (1931).
Nomenclature of Synthetic Rubbers HARRY L. FISHER U. S. Industrial Alcohol Company, Stamford, Conn.
A brief history of synthetic rubbers and of synthetic rubberlike substances is given, together with an outline of the reasons for the continued use of the term “synthetic rubber,” especially for the rubberlike polymers of butadiene and its derivatives, including chloroprene. Recent and new class terms for rubberlike substances are given and their uses discussed. The new term “elastomers” is suggested to cover all rubberlike substances, “elastoprenes” for the diene polymers, “elastolenes” for the polyisobutylenes, and “elastothiomers” for the polyethylene sulfides (Thiolrol). It is also suggested that Stevens’ term “elastoplastics” be used for the growing class of rubberlike plastics such as plasticized vinyl chloride (Koroseal), certain polyacrylic esters, etc. “Plastomer” is used for the true and the thermosetting thermoplastics. A classification of all rubberlike substances is tabulated.
IXTY years ago, synthetic indigo, a dream of organic chemists, became a reality. Thirty years ago the increase in the knowledge of the chemistry of rubber made organic chemists dream also of synthesizing that important natural product. However, rubber or, more specifically, the rubber hydrocarbon has not yet been synthesized (8) in spite of the tremendous amount of time and effort already expended on this intriguing problem. But in scientific journals, books, newspapers, and advertisements there is much that is published about “synthetic rubbers.” Indigo was synthesized and there is no question about speaking of synthetic indigo. Since rubber has not been synthesized, why do we hear so much about synthetic rubbers? Are there any other names which could be used to describe the various “synthetic rubbers” and other rubberlike
products? These are the questions which will be discussed in this paper. Indigo is crystalline and can be purified easily; the rubber hydrocarbon can be crystallized only under very special conditions, cannot be distilled, and therefore is not easy to purify. Indigo has a comparatively low molecular weight which can easily be determined; the rubber hydrocarbon is an elastic polymer, the molecular weight of which is very high and cannot be determined with precision. A determination of the identity of the natural and synthetic samples of indigo can readily be made, but with rubber it is almost impossible with our present methods to show the absolute identity of two specimens, although it is possible for all practical purposes to do so.
History of Synthetic Rubber As long ago as 1860 Williams (42) separated isoprene as a definite compound among the products of the destructive distillation of rubber. Fifteen years later Bouchardat (4) recognized the probable relation of isoprene to rubber and actually converted it to a rubberlike solid. I n 1882 Tilden (38) discussed the possible industrial significance of the polymerizability of isoprene, provided it could be obtained commercially from a source other than natural rubber; in 1892 he reported (39) that isoprene which had been prepared from turpentine had spontaneously polymerized to a rubberlike product-he said “rubber.” Early in the present century Kondakoff (20) found that 2,3-dimethylbutadiene, a homolog of isoprene, slowly polymerizes to a rubberlike product, and similar observations were made concerning piperylene or 1methylbutadiene (16, 37), and butadiene itself (14, 21). Commercial quantities of “synthetic rubber” were manufactured in Germany during the World War from 2,3-dimethylbutadiene; the product was known as methyl rubber (13,30,41). There was a lull in synthetic rubber research until the rise in the price of rubber in 1925 furnished a stimulus to further work. In the present decade wonderful strides have been made, and now large quantities of “synthetic rubber” are being made from butadiene in Germany and Russia, and from a chloro derivative of butadiene (chloroprene) in this country. These “synthetic rubbers” are all prepared by processes of polymerization, and they bear a strong resemblance to natural rubber. They differ chemically from natural rubber,
INDUSTRIAL AND ENGINEERING CHEMISTRY
VOL. 31, NO. 8
‘ Butadiene rubbers:
Sodium butadiene rubber, Russia (1, 16) Buna rubbers, Germany (19) Piperylene rubbers (16) Isoprene rubbers: Polyprene: natural rubber Elastoprenes Sodium isoprene rubber (16) (derivatives of butadiene) . Heat-polymerized isoprene rubber (15) Dimethylbutadiene rubbers: Cold polymer: methyl rubber H (13, 41) Heat polymer: methyl rubber W (13,41) Haloprene rubbers: Polychloroprene rubber: neoprene (10) ELASTOMERS Polybromoprene rubber (9) Polymers, such as polyisobutylene, formed in the presence of a catalyst-e. g., boron trifluoride: Elastolenes Vistanex, Oppanol B (6, 31) Elastothiomers Polyalkylene sulfidea: Thiokol, Perduren ($2, 27) ( Rubberlike polymers of acrylic and methacrylic esters: Acranal, Plexigum (19) Rubberlike mixed glyptals (43) Plasticized polyvinyl chloride: Koroseal, Igelite, Mipolam (7, 18) Polyvinyl acetate, above 40’ C. (40) Elastoplastics Polystyrene, above 6 5 O C., and when partially solvated ($4, 38, 40) Polyarylenethylenes or polyxylenes: AXF, from benzene, ethylene chloride, and aluminum chloride
Pdlyphosphonitrilic chloride (PNCh)z, an inorganic rubber (23, $9,86) True thermoplastics PLASTOMERS Thermosetting plastics
Shellac, polystyrene, polyvinyl acetate, celluloid, cellulose acetate Bakelite, glyptals, formaldehyde-urea polymers, acrylic resins
The Term “Synthetic Rubber”
“Artificial” is a perfectly good word, but unfortunately it carries a connotation that is not always desirable. Artificial flowers, artificial light, artificial gems, and artificial teeth illustrate this point. Artificial means “produced or modified by human skill or labor, in opposition to natural.” The building u p of an artificial rubber or a substitute for rubber is so much like a regular chemical synthesis of a desired product that the term “synthetic rubber” appears to be a good and appropriate name. It is of interest that a somewhat similar situation has arisen in the nomenclature of artificial fibers. The name “rayon” was given to fibers and threads made from viscose t o replace the term “artificial silk.” At present there are several kinds of rayon made from different cellulose derivatives, and similar fibers are made from casein and resinous products; the latter are also sometimes called “rayon.” I n other words, rayon has become the name of a type of fiber. Similarly “synthetic rubber” covers a type of material. Houwink (16) gave the following broad definition of a rubberlike material: “An organic material may be called a rubber when it shows a high elasticity of 100 per cent or more a t room temperature, and when it does not lose this property upon storage at room temperature during considerable periods.” This definition was criticized by Stevens (35) partly because it includes substances other than real rubber. Midgley (24) discussed the question as follows:
We can see, therefore, that the use of the term “synthetic rubber” has been widespread, although strictly speaking it is not properly used. However, when the situation is considered carefully, there does seem to be justification for it. If a piece of ‘(syntheticrubber” is handed to a man, he will note its similarity to natural or vulcanized rubber and quickly say, “That’s rubber.” If it is not natural or vulcanized rubber, then what should It be called? It may be called a substitute rubber or properly an artificial rubber. Harries (16),who was one of the foremost workers in the field of synthetic rubber, wrote a book covering his researches, and he was careful a t that time (1919) to use the German word kiinstlichen (artificial) rather than synthetischen (synthetic).
It is impossible at the present time to define synthetic rubber in chemical terms.. . . .Expressed in physical terms, the simplest definition is, “thpse substances which possess the physical properties of rubber.” Such a statement is functional, and should be revised in terms defining a uni ue physical property of rubber. Several organic substances of %gh molecular weight may be stretched to many times their original lengths, i. e., gums, tars, waxes, jellies, etc.; but only rubber forcibly retracts to substantially its original size and shape after such stretching. Hence the definition becomes: “Synthetic rubbers are those organic substances which possess the property of forcibly retracting to a proximately their original size and shape after being greatly gistorted, i. e., such as being stretched x per cent of their original lengths.” Here 5 is some arbitrary value. It should be over 100, probably 400, possibly 600, but certainly not higher.
but most of them, especially the German Buna and the American Neoprene, have physical properties which in the vulcanized state make them superior to similar products from natural rubber; i. e., they are more resistant to the action of oils, fats, solvents, heat, air, sunlight, and, in some cases, abrasion. There are also other synthetic rubberlike materials, and some of them are called “synthetic rubbers,” although they are not related chemically to natural rubber or to the polymeric derivatives of butadiene-namely, methyl methacrylate rubberlike polymers, polyalkylene sulfides (Thiokol), polyisobutylenes (Vistanex, Oppanol), plasticized polyvinyl chloride (Koroseal), polystyrene above 65” C., polyvinyl acetate above 40” C., the inorganic rubberlike polyphosphonitrilic chloride, etc. They also must be classified. All the synthetic substances so far mentioned have properties resembling rubber; they have been described in the literature not only as “synthetic rubbers” but also as “synthetic elastics,” “rubberlike polymers,” “rubberlike substances,” “products with rubberlike properties,” “plastic rubberlike materials,” “rubbery polymers,” etc. Rubber is also a plastic as well as an elastic substance and so are these other substances, but they all have these properties to different degrees.
NOTES os TABLE 11. STRUCTURAL Butadiene
CHI - CH CH - CH=CHz CH3
CHz= C- CH
H3C CHI I 1 CHz= C- C = CHz
c1 CHz = C - CH = CHz
--CHZ-CH=CH-CHI--CHZ-CH =CH-CHz-The Russian synthetic rubber is a sodium polymeri~edbutadiene. The numbered Buna rubbers (Buna 32, etc.) are also sodium polymers. Buna S consists of mixed polymers of butadiene and styrene, polymerized in the form of an emulsion. Buna N similarly consists of mixed polymers of butadiene and acrylic nitrile (CHz = CH-CN) prepared in the form of an emulsion. CH3 CHs I I - CH = CH - CHz--CH - CH CH - CHz--CH CHa CH3
I --CHz - C
CH - CHz-CHzC = CH - CHFIn the natural rubber hydrocarbon, the methyl groups occur regularly along the chain. In the synthetic isoprene rubbers, the methyl groups occur more or less irregularly, since, whgn stretched, they do not give the x-ray fiber diagram. These unsymmetrical polymerides, judging from both chemical and x-ray results, have groupings somewhat as follows: CHa CHa CH3 I I I -_ CHz- C = CH- C H y C H z - CH = C- CHz-CHzC = CH-CHHac CH3 Hac CH3 I I I I -- CHz-C‘= C-CHs---CHz-C=C-CHz-The methyl groups occur regularly along the chain, as shown by chemical evidence, and this polymeric product when stretched gives an x-ray fiber diagram. c1 c1
--CHz- C = CH - CHz---CH2-
Structure of the product is not known. The unsaturation is very low and probably occurs only in the “end molecule” of isobutylene. It is presumed that Oppanol B is the same or a similar substance. When stretched it gives an x-ray fiber diagram ( 6 ) .
CH3- C = CHz
C = CH - CHIn this polymeride the chlorine atoms evidently occur regularly, since when stretched it gives an x-ray fiber diagram.
SUBSTANCES ENUMERATED IN TABLE I
Probable or Possible Structures of Polymers
Starting Materials CHz = CH - CH = CHz
Ethylene chloride sodium polysulfide
CHzCl - CHzC1 + S’aS,
CHz = CH - COOCHD
I1 I1 HS - CHzCHz - S -S - CHzCH-S - S - . . . . . - CHzCHz - SH Similarly with 2,2’-dichloroethyl ether, ClCHzCHz- 0 - CHzCHzCl, etc. II
CHz- CH-CHz-CH-CHzI I CH30CO CHaOCO
CHz = C - COOCHD
I Mixed glyptals “ 0 Phthalic anhydride
+Mixed esters of high - molecular weight -
CH20H+ Hz? - ‘\O CHzOH HzC-C’
0 Ethylene Succinic glycol anhydride
CHz = CH - OCOCHa
OCOCHs I CHz - CH-CHz-
c1 I CH-
0 vn v“3 OcH=CHz *() 0 0 0 I
Styrene (vinyl benzene)
CHz = CHCl
c1 Vinyl chloride
CH-CHzCH-CHzThis formulation is according t o Staudinger (33)
-CHzCH-CH-CHz-CHz-CH--CH-CHThis is according to Midgley et al. (66) Ethylene chloride benzene
Phosphorus pentachloride ammonium chloride
CHzCHz - CBHh-CHzCHzCsHa-CHzCHzc&4The position of attachment on the benzene nucleus is not known; therefore, only the molecular formula is used. c1 c1 (PNClZ),
-pI = N-p= I
c1 ci Phosphonitrilic chloride
INDUSTRIAL AND ENGINEERING CHEMISTRY
Bridgwater (5) describes “synthetic substances with rubberlike properties” as substances that resemble rubber in the simple property of extensibility or deformability under moderate loads, coupled with a tendency to recover their original form when the load is removed, although not necessarily to a degree comparable to the recovery exhibited by natural rubber. The question of the underlimit of extensibility and of the rate and extent of retraction of a substance to bring it into the class of synthetic rubber or rubberlike materials has never been settled. A decision by an international agreement of organizations interested in these materials and, in fact an international effort to bring order into the entire subject of rubber terminology, as already suggested by Dawson ( I I ) , would be helpful.
VOL. 31, NO. 8
Another suggestion is “caoutchoid” or “couchoid” by Patterson ($8). He points out that the word rubber is English and not an international word, and that therefore rubberoid (rubberlike) would not be generally acceptable. Accordingly he uses the word caoutchouc as the basis of a better derivative and suggests the words given. Since caoutchoid has “an abominable spelling” he thinks that the unpronounced letters could be dropped to form the simple term “couchoid.” These suggestions are good, and only time will tell how much they will be used. To the writer “collastic” seems to emphasize the colloidal property in preference to the more important elastic property of rubber. “Elastoplastic” has much to recommend it although i t has five syllables and is not easy to speak. “Couchoid” has an excellent derivation but it, too, is not easy to say.
The Names Rubber, Isoprene, etc. Rubber was given its name because it has the property of rubbing out pencil marks, according to a record left by Joseph Priestley in 1770 ( 2 ); but the word was probably in use before that date. Languages other than English use words which were derived from the native words caa o-chu or cahuchu, meaning weeping tree-namely, caoutchouc in French, Kautschuk in German, etc. “Elastic gum” has been used in English, and similar words appear in Spanish and Italian, but rubber is not a true gum and therefore this is not a proper term. The word “rubber” stands for more than a single chemical compound or a typical natural product. It is also used for vulcanized rubber and articles made from it-overshoes, elastic bands, etc. As Stevens (34) says, “It is not an elegant word, and its derivation is almost ludicrous in contrast with its modern applications.” It is also not an international term. There is a question, therefore, whether i t is advisable to use the word in a general term covering all types of rubberlike materials. Weber named the rubber hydrocarbon “polyprene,” which was coined from polymer and isoprene. Isoprene was named by Williams (42) who states: “I have given the substance thus examined the name of isoprene. It would have been more grateful to me to have retained one of the names given by the previous observers, if that course had been possible; but Himly has not named the fluid discovered by him boiling between 33’ and 44”,and the term caoutchhne having been applied by Bouchardat to a fluid boiling a t 14.5’, I could not adopt it; moreover, it is too like caoutchine.” The suffix prene has also been used in chloroprene which is structurally similar to isoprene, with a chlorine atom in the place of the methyl group in position 2 of butadiene. Although the origin of the suffix prene is not known, it has been associated with rubber for many years and therefore is worth keeping in future names.
Recent Class Terms for Rubberlike Substances Although there is some justification for the term “synthetic rubber,” it seems best that it be used chiefly in connection with products that are related chemically to natural rubberthat is, to the various derivatives of butadiene. Usage, however, will determine this. At any rate there is a need for a single term which can be used to cover all rubberlike products. The subject of the use of the words “synthetic rubber” and the need for a single term was discussed recently in the correspondence of Stevens (35), Barron (S), and Naunton (26). I n this correspondence the most desirable words suggested are “collastics,” from colloid and elastic, by Barron, and the selfexplanatory “elastoplasts” by Stevens, or “elastoplastics” as modified by Naunton. These have good derivations and are worthv of consideration.
New Suggestions The writer also comes into the discussion with new suggestions, the first of which is “elastomer.” This word is reminiscent of isomer, electromer, metamer, and polymer, and it is hoped that it may prove of general service. I n a conversation on this subject, the writer’s colleague, W. C. Moore, suggested “plastomer” to cover the nonelastic plastic substances, and the writer presents elastomer to cover the elastic or rubberlike substances. Elastomer is easy to speak, has a scientific derivation, and emphasizes the elastic properties of all these substances. For a general term to cover the rubberlike polymers of butadiene and its derivatives, including chloroprene, the writer suggests “elastoprenes” ; for the polyisobutylenes, “elastolenes” ; and for the polyethylene sulfides, “elastothiomers.”l The derivation of each of these terms is obvious. He further suggests that Stevens’ term “elastoplastics” be used as the name of that growing class of rubberlike plastics which includes the rubberlike glyptals and polymethyl methacrylates, plasticized vinyl chloride, etc.
Classification Jacobs (17) recently classified synthetic rubbers under the following four headings: (a) halo- or halogenorubbers (Neoprene), (b) alternative or eo-rubbers (Buna), ( c ) thiorubbers (Thiokol and Perduren), and (d) plasto- or resorubbers (vinyl polymers and other unvulcanizable thermoplastic polymers made from hydrocarbons). The classification given in Table I is offered for all the synthetic rubbers and rubberlike polymers and plastics. Table I1 contains structural notes on the substances mentioned in Table I. The long bonds in the structural formulas of the polymers are used to indicate the places where the original molecules are joined together. This article is not presumed to be the last word on the subject. It is written with the hope that it will help to clarify the present confused situation in regard to the use of the term “synthetic rubber,” and to help classify all the substances with rubberlike properties. It is also hoped that the article will stimulate more thinking on the subject and soon bring order out of the present nomenclatural chaos. After this paper was presented the author accidentally came across the terms “lastic” and “synlastic,” used by Ellis (12). Also, his attention was called to the proposals of Kindscher (18) in which crude rubbers, synthetic rubbers (from butadiene and its derivatives, Thiokol, Neoprene, etc.), and rubberlike polyvinyl compounds, polyisobutylenes, etc., are classified under the terms Kautschukgeqe, Kautschukoide, and Gummoide. 1 In t h e paper as originally presented, the polyethylene sulfides were called “thiolastics.”
INDUSTRIAL AND ENGINEERING CHEMISTRY
Acknowledgment The writer is grateful to E. J. Crane, H. E. Howe, H. J. D’Innocenzo, W. C. Moore, and A. M. Patterson for their interest, encouragement, and helpful suggestions.
Literature Cited (1) Akob~hanov,Rubber Chem. Tech., 8,430 (1935). (2) Barker, Rubber Age (N. Y . ) ,43, No. 2, 103 (May, 1938). Chem. I n d . , 55,844 (1936); I n d i a Rubber J., 92, (3) Barron, J . SOC. 542 (1936). (4) Bouchardat, Compt. rend., 80, 1446 (1875)and 89, 1117 (1879); Bull. SOC. chim., 24, 108 (1875). (5) Bridgwater, I n d i a Rubber World, 44, No. 1, 21 (Oct., 1938). (6) Brill and Halle, Naturwissenschaften, 26, 12 (1938); Rubber Chem. Tech., 11, 687 (1938). (7) Brous and Semon, IND. ENCI.CHEM.., 27,667 (1935). (8) Carothers, Ibid., 26, 30 (1934). (9) Carothers, Kirby, and Collins, J . Am. Chem. SOC., 55,789(1933). (10) Carothers, Williams, Collins, and Kirby, Ibid., 53, 4203 (1931). (11) Dawson, Proc. Rubber Tech. Conference, London, 1938, 1003. ENG.CWEM., 28, 1138 (1936). (12) Ellis, IND. (13) Gottlob, I n d i a Rubber J . , 58,305,348,391,433 (1919);“Technologie der Kautschukwaren,” 2nd ed., p. 211, Brunswick, Germany, Friederich Vieweg & Sohn, 1925. (14) Harr!os, Ann., 383, 157 (1911). (15) Harries, “Untersuchungen uber die naturlichen und kunstlichen Kautschukarten,” 1919. (16) Houwink, I n d i a Rubber J., 92,455 (1936). (17) Jacobs, Caoutchouc & gutta-percha, 35,35 (1938). (18) Kindscher, Kautschuk, 14, 140 (1938); Rubber Age (London), 19,286 (1938).
(19) Koch, Rubber Chem. Tech., 10, 17 (1937); paper presented a t 97th Meeting of A. C. S., Baltimore, 1939. (20) Kondakoff, J . prakt. Chem., 64,109 (1901). (21) Lebedeff, J . Russ. Phys. Chem. SOC.,42, 949 (1910); Chem. Zentr., 1910,11, 1744. (22) Martin and Patrick, IND. ENG.CWEM.,28, 1144 (1936). (23) Meyer, Trans. Faraday SOC.,32, 148 (1936); Rubber Chem. Tech., 9, 422 (1936). (24) Midgleu, “Chemistry and Technology of Rubber,” 678 (1937). (25) Midgley, Henne, and Leicester, J. Am. Chem. SOC., 58, 1961 (1936). (26) Naunton, J . SOC. Chem. I n d . , 55,297,328 (1936). (27) Patrick, Trans. Faraday SOC.,32, 347 (1936). (28) Patterson, A. M.,personal communication. (29) Schenck and Romer, Ber., 57, 1343 (1924). (30) Schotz, “Synthetic Rubber,” London, Ernest Benn, 1926. (31) Schwartz, Kunststofe, 29, 9 (1939); I. G. Farbenindustrie, British Patent 432,196 (1935); and other patent literature. (32) Shinkle, Brooks, and Cady, IND. ENQ.CHEM.,28,275 (1936). (33) Staudinger, Ber., 59, 3036 (1926); 62,241,2406 (1929). (34) Stevens, J , SOC.Chem. Ind., 55, 814 (1936). (35) Ibid., 55, 276,328,443,814 (1936). (36) Stokes, Am. Chem. J . , 17,275 (1895); 19,782 (1897). (37) Thiele, Ann., 319, 226 (1901); Bayer & Co., German Patent 235 686 I1 909). (38) Tilden, Chem. News, 46,120 (1882). (39) Ibid., 65,265 (1892). (40) Whitby, Trans. Inst. Rubber Ind., 5, 184 (1929); 6,40 (1930). ENQ.CHEM.,25, 1204, 1338 (1933). (41) Whitbv and Katz. IND. (42j Williams, C. G.,Trans. Roy. SOC.(London), 150, 241 (1860); Proc. Roy. SOC.(London), 10, 516 (1860); J . Chem. SOC., 15, 110 (1862). (43) Wright, Chem. & Met. Eng., 39,438 (1932). - - - I - - -
Svnthetic Elastic Polvmers in the Cable Industrv J
R. A. SCHATZEL AND G.W.CASSELL General Cable Corporation, Rome, N. Y. The position of plastic materials in the ca,ble industry is dependent upon cost and properties. Plastics, irrespective of costs, are being used where necessary properties cannot be obtained with the older, more commonly used materials. As might be expected, many of the first applications will be discarded when cost and service records are weighed one against the other. On the other hand, rapid and constant improvements in these new materials will greatly extend their use. Increased consumption will lower their present costs and permit applications which are now too expensive. At the present market price of rubber, the plastics and rubberlike materials discussed above are from three to seven times more expensive. This increase in cost can be justified only by a much longer life in service. If, through greater resistance to deterioration from elements met in service, these materials improve the dependability of electrical service by freedom from shutdown and need of replacement, the advantage in their use will justify a larger original investment. All of the materials discussed have certain weaknesses, but it is reasonable to believe that a few of them will be improved to make a more balanced
composition. It may be through the use of better plasticizers or it may result from mixtures of various synthetic resins. In any event, if progress is as rapid in the next decade as it has been in the past ten years, there will be a great many useful synthetic materials for the cable industry.
HE place of synthetic elastic polymers in the cable industry cannot yet be evaluated, and no final conclusions can be drawn from a survey a t this time. The development in this field has been very rapid and is by no means complete. However, a useful purpose may be served and some direction given to those interested in the development and manufacture of the basic materials, by setting forth the ideas of those who are using these materials for special applications. They have a place in the cable industry, but the extent will be determined by the following considerations: 1. Whether economies in the cost of cable, or cable operation, result in the replacement of present insulating or protecting materials now in use. 2. Whether these materials will provide satisfactory products where none exist at present. 3. Whether these substances will complement present materials to form an improved product.
The materials covered by this brief review are those which are manufactured on a commercial basis and have been more or less widely used in this country or abroad. For the sake of